**BIBECHANA **

**A Multidisciplinary Journal of Science, Technology **
**and Mathematics **

ISSN 2091-0762 (online)

Journal homepage: http://nepjol.info/index.php/BIBICHANA

### Anomaly in energetic and structural properties of MgSn

### liquid alloys

A. Kumara∗∗∗∗, I. S. Jhaa, B. P. Singhb a

Dept. of Physics, M.M.A.M Campus Tribhuvan University, Biratnagar, Nepal. b

University Department of Physics ,T.M. Bhagalpur University, Bhagalpur, Bihar, India

*Article history: Received 1 November 2010; Revised 15 November 2010; Accepted 18 November 2010 *

Abstract

The observed asymmetry in the properties of mixing of MgSn alloy in molten state is successfully explained on basis of the quasi-lattice model. It has been utilized to determine the free energy of mixing, entropy of mixing, heat of mixing, the concentration- concentration structure factor in long wave-length limit [Scc(0)] and the Warren Cowley short range order parameter (α1) of

MgSn alloy in molten state at 1073 K. The analysis suggests that heterocordiantion leading to the formation of chemical complex Mg2Sn is likely to exist in the melt but is of a weakly interacting

in nature. The interaction energies between the species of the melt are found to depend considerably on temperature and the alloy is more ordered towards Mg rich region

**Keywords: ** **Quasi-lattice model; Binary alloys; Short range order parameter; **
**Asymmetry**

**1. Introduction **

A large number of binary alloys specially the compound forming alloys exhibit interesting behaviour as a function of concentration as regards the thermodynamic [1] and electric properties [2, 3]. The properties of mixing are not symmetrical about the equiatomic composition-deviating maximally from those of ideal alloys. Some of the alloys also depict metal - non metal transition across narrow band of concentration. The liquidus lines are usually S-shaped and the heat of mixing and excess free energy of mixing are large negative quantities at one or other concentrations [4- 6]. The anomalous behaviour of these liquid alloys still demands extensive theoretical investigation.

The properties of mixing of MgSn alloy is of interest as various properties of it show anomalous behaviour as the function of concentration. The liquidus line is endowed with two eutectics in the terminal region of concentration with the bump around the stoichiometric

∗

composition of Mg2Sn. The large value of viscosity [7] and the analysis of the radial distribution

function [8] indicate that unlike atoms attract, with the interaction being greatest at the composition Mg2Sn.The properties of mixing show asymmetry around the equiatomic

composition for MgSn alloy also.

There are so many models such as pseudo potential theory [9, 10], hard sphere model [11- 14], the conformal solution model [15] etc. to study the alloying behaviour of liquid alloy. But in the present investigation we have used quasi-lattice model developed by Bhatia and Singh as it is successful in investigating both the thermodynamic properties and microscopic structure [16, 17]. On the basis of this model we have calculated the thermodynamic quantities such as free energy of mixing, excess entropy of mixing, and heat of mixing. To understand the microscope structure of the alloy we have calculated concentration-concentration fluctuation in the long wave-length limit [Scc(0)] and the short range order parameter [α1]. The phenomena of compound

formation and segregation can easily be interpreted through the study of Scc(0) and α1 [18-26].

In section 2 the general formulation of quasi-lattice model are summarised to simple expressions. Section 3 deals with the results and discussions. Section 4 provides the conclusion.

**2. Theory **

The quasi-lattice chemical model envisages the existence of chemical complex [Aµ Bν] where A and B are constituent species and µ and ν are small integers, µA + νB AµBν.

The grand partition function is solved by assuming that the energy of a given nearest bond is different if it belongs to the complex than if it does not. With this consideration the expression for excess free energy of mixing comes out to be

dc ln T NK

G c

o B XS

M =

### ∫

γ (1)where N is the total no. of atom in the alloy ‘c’ the concentration of atom A T the absolute scale temp., KB the Boltzman constant and γ is the ratio of the activity co-efficient of atom A to B.

The solution of equation (1) leads to

### [

AB AB AA AA BB BB### ]

XS

M Nc(1 c)

G = − ω+φ ∆ω +φ ∆ω +φ ∆ω (2)

where ω's are ordering energy and φ is some constant given by

KBT φµ, ν = ∆ωΑΒ[2β (µ+1, ν) – 2β (µ, ν+1) + β (2µ, 2ν–1) + β (2µ – 1, 2ν)] + ∆ωΑΑ[β (2µ–2, 2ν + 1)

– 2β (µ, ν+1) + ∆ωΒΒ [2β (µ+1, ν) – β (2µ + 1, 2ν–2)] (3)

for Fe-Si liquid alloy

A = Mg, B = Sn, µ = 2, ν = 1

φAB(c) =

+ −

+ 2 3 _{c}4

2 1 c 3 5 c c 6 1

(4)

φAA(c) =

− +

− 2 c4

4 1 c 2 1 c 4 1

(5)

φBB(c) = 0 (6)

Using eqn. (4), (5) and (6) in eqn. (2),

XS 2 3 4 2 4

M AB AA

1 5 1 1 1 1

G N c(1 c) c c c c c c c

6 3 2 4 2 4

= ω − + ∆ω _{} + − + _{}+ ∆ω _{}− + − _{}

(7)

The free energy of mixing of complex forming binary alloy

GM = G_{M}XS+RT

### [

clnc+(1−c)ln(1−c)### ]

(8)The excess entropy of mixing is given by P XS M XS M ) dT dG ( S =−

)] c ( ) ( dT d ) c ( ) ( dT d ) c ( ) ( dT d ) c ( dT d [ N

SXS_{M} =− ωφ + ∆ω_{AB} φ_{AB} + ∆ω_{AA} φ_{AA} + ∆ω_{BB} φ_{BB} (9)

where φ(c) = c(1–c).

xs

M M

S =S −R[c ln c (c 1) ln(c 1)+ − − (9a)

From standard thermodynamic relations, the heat of mixing

HM = GXS_{M} +TSXS_{M} (10)

To understand the nature of atomic order in the binary liquid alloy it is instructive to study the behaviour of the long wave-length limit of the concentration-concentration structure factor [Scc(0)] (16, 17) given as

Scc(o) =

N , P , T 2 M 2 B c G T

NK _{}

∂

∂ _{ } _{ (11) }

where GM is free energy of mixing.

Using eqn. (7), (8) and (11)

Scc(o) =

### [

AB AB AA AA BB BB### ]

B 2 T K ) c 1 ( c 1 ) c 1 ( c φ ′′ ω ∆ + φ ′′ ω ∆ + φ ′′ ω ∆ + ω − − + − (12)

where φ ′′i,j= (i,j A,B) dc d 2 j , i 2 = φ

The experimental determination of Scc(0) poses more difficulty, but it can be determined

from measured activity data and it is usually considered to be experimental values. The warren-Cowley short-range order parameter (α1) [26, 27]. Can estimated from the knowledge of Scc(0) as

α1 =

1 ) 1 z ( S ) 1 S ( + − −

, S = ) 0 ( S ) 0 ( S id cc cc ) 0 (

Sidcc = c (1– c) and z is co-ordination number z = 10 has been taken for our calculation.

**3. Results and Discussions **

**3.1 Free energy of mixing **

The energy parameters used for the calculations of the free energy of mixing for MgSn liquid alloys are has been determined from experimental values of GM (1) in the concentration

range from 0.1 to 0.9 by the method of successive approximation. The coefficient (∆ωBB) = 0

since ν = 1. The remaining two parameters are found to be

B

5.0, K T

ω

= − AB B

0.86 K T

∆ω

= − and AA B

0.47 K T

∆ω = −

Thus equation (7) and (8) are used to compute free energy of mixing (GM/RT) of MgSn

liquid alloy.

The theoretical and experimental values of free energy of mixing for MgSn liquid alloy is shown in figure 1. The theoretical result is in good agreement with experimental values in the terminal regions of concentrations cMg = 0.1 to 0.3 and 0.8 to 0.9, in which the liquidus line is

rise with the bump at cMg = 0.66. The experimental value shows value of GM/RT= -2.316 at cMg =

0.6 but our theoretical result shows minimum GM/RT= -2.0714 at cMg = 0.51. The theoretical

analysis of free energy of mixing shows that in liquid state MgSn is a weak interacting system.

**3.2 Entropy of mixing **

To determine the excess entropy mixing for MgSn liquid alloy we need the temperature derivatives of interaction parameters in Eq. (9). The observed values of SX

M

S are used to obtained the temperature derivative by successive approximation method. It is notice that the temperature

derivative of ωAA is negligibly small so we set the dT

d

(ωAA) = 0 and also dT

d

(ωBB) = 0. The

remaining parameters are found to be

2 . 0 dT d K

1

B

− = ω

AB

B d 1

0.03

K dT

ω

= −

The excess entropy of mixing is calculated using Eqs.(9) and (9a) to evaluate SM. The

theoretical and experimental values of
R
S_{M}

against cMg are plotted in figure 1. The theoretical and

experimental values are in excellent agreement. Both show minimum at cMg =0.6.

**3.3. Heat of mixing **

The heat of mixing for MgSn liquid alloy has been computed from Eq. (10) using the

same values of dT dω

and dT

dωAB _{. The plot of }
RT

HM _{ versus c}

Mg at 1073K is depicted in figure 1. The

theoretical and experimental values are in good agreement. The theoretical and experimental

**Figure: ** Free energy of mixing

### (

GM /RT### )

, heat of mixing (HM /RT) andresults show almost the same nature as shown by the free energy of mixing. Again the theoretical results are good agreement in terminal regions of concentration but do not agree so well in the intermediate region of concentration.

**3.4. The concentration-concentration structure factor [Scc(0)] and short range order **

**parameter (**αααα**1) **

The theoretical values of Scc(0) computed from Eq.(12) using the same energy

parameters and experimental values along with the ideal values are shown in figure 2. The theoretical values of Scc(0) are in good agreement with the experimental values. Scc(0) can be

used to understand the nature of atomic order in binary alloys. At the given composition if Scc(0)

< Sidcc(0), ordering in liquid alloy is excepted and if Scc(0) > Sidcc(0), there is tendency of

segregation. We find that there is a clear dip at cMg = 0.7 showing that Mg2Sn is most ordered at

this concentration.

**Figure 2: **Upper part concentration fluctuation in long wave-length limit
[Scc(0)] for MgSn liquid alloy at 1073 K at different concentrations of
Mg. [––––] theoretical, [oooo] experimental. Lower part short range order
parameter (α1) versus cMg.

The knowledge of α1 provides an immediate insight into the nature of the local arrangement of

atoms in the mixture. The minimum possible value of α1 is –1 and it implies complete ordering

of unlike atom paring at nearest atoms. On the other hand the maximum value of α1 is +1, which

implies complete segregation leading to the phaseseparation and α1= 0 corresponds to a random

distribution of atoms. Figure 2 show that α1 is negative throughout showing that α1 MgSn is an

ordered system of unlike atom pairing at all concentration. α1 is found to be minimum at cMg =

**4. Conclusion **

In present work, we have used quasi-lattice model and calculated the pair wise interaction energy for MgSn liquid alloy at 1073 K. These were used to estimate the thermodynamic properties and concentration fluctuation in long wavelength limit of MgSn liquid alloy. Computed values of Scc(0) and α1 suggest that there is a tendency towards unlike atom pairing

(Mg-Sn) over the whole range of concentration. Our theoretical analysis shows that the complex Mg 2 Sn is present in the molten state of MgSn alloy.

**References **

[1] R. Hultgren P. D. Desai, D. T. Hawkins, M. Gleisser and K. K. Kelley. Selected values of the Thermodynamic Properties of Binary alloys. ASM, Metal park ohio, 1973 (871). [2] G. Busch, H. N. Guntnerodt, in Ehrenreich, F. Seitz, D. Turnball (Eds) solid state

Physics, Academic, New York ,**29** (1974) 1235.
[3] S. Takeuchi, K. Murakami, Sci. Rep. RITU, **25** (1974).

[4] P. Chiux and H. Rupersberg, J. Phys (Les Ulis. Fr.) ,C8 (Lam4) **41** (1980) 145.
[5] P. Lamperter, W. Martin and S. Steeb, J. Non Cryst. Solids, **61** (1984) 279.
[6] B. C. Anusionwu, Pramana, J. Phys., **67** (2006) 319.

[7] V.M. Glazov, S.N. Chizhevskaya and N.N. Glagoleva, Liqs. Semicondutors (New York Paenum), (1969)277.

[8] S.Steeb and H. Entress, Z. Metallik, **57**(1966)803.

[9] W. A. Harrison Pseudo potential in the theory of metals, Benjami New York, (1966). [10] V. Hein, Solid state physics ,Academic New York, (1970).

[11] E. Theile, J. Chem. Phys, Lett., **39 **(1963) 474.
[12] J. Libowitz, Phys. Rev. A,**133** (1964) 895.

[13] T. E. Faber, Introduction to the theory of liquid Metals Cambridge University Press, Cambridge, (1972).

[14] M. Shimoji, Liquid Metals ,London Academy London ,(1977).
[15] H. C. Longuet Higgins, Proc. Roy. Soc., A **205** (1951) 247.
[16] A. B. Bhatia and R. N. Singh (Phys. Chem Liqs., **11** (1982) 343.
[17] A. B. Bhatia and R. N. Singh (Phys. Chem. Liqs., **13 **(1984) 177.
[18] D. Adhikari, I.S.Jha and B.P.Singh, Physica B, **405**(2010)1861.

[19] A. B. Bhatia, W. H. Hargrove and N. H. March, J. Phys. ,C**6 **(1973) 621.
[20] J. A. Alonso, and N. H. March Physica B,1**14** (1982) 67.

[21] E. A. Guggenheim, Mixtures, Oxford University Press, Oxford, (1952).

[22] N. K. P. Singh, I. K. Mishra and V. N. Singh J. Phys. Conds. Matter ,**2 **(1990) 8445.
[23] R. N. Singh and L. C. Prasad Phys. Chem. Liqs. ,**22** (1990)1.

[24] S. K. Chatterjee and L. C. Prasad, Indian J. Pure App. Phys., **42** (2004), 279.

[25] N. K. P. Singh, R. N. Singh and R. B. Choudhary, J. Phys. Conds. Matter, **3 **(1991) 5345.
[26] J. M. Cowley, Phys. Rev. 77 (1950) 667.